March 2012, Volume 8, Issue 3
Published by AEGIS Communications
Adhesives: Newer Is Not Always Better—Part 2
Part 2 offers an update and overview of self-etch adhesive systems and addresses postoperative sensitivity associated with total-etch adhesives.
Part 1 of this article discussed etch-and-rinse adhesives—the so called fourth and fifth generations—with particular attention to methodology in order to maximize their performance. The clinician must be aware of the type of solvent used, and whether the system is a filled resin, as these factors modify the application technique. Because postoperative sensitivity has been identified as a possible result with these etch-and-rinse adhesives, Part 2 addresses how to clinically minimize—or totally eliminate—this problem. The authors also offer an overview of the self-etch adhesive systems and their current status in restorative dentistry. This second article also looks at the lack of longevity of dentin bonding, which may be affected by matrix metalloproteinases (MMPs), and how current research may offer insights on ways current clinical techniques and adhesive systems can be changed to address this issue.
Glutaraldehyde is a very effective fixative, or flocculating agent, which has the ability to create a cross-linked protein plug inside the dentinal tubules. It has been accepted extremely well by dentists as a material that reduces or totally eliminates tooth sensitivity.1 Schupbach2 has shown that after topical application of glutaraldehyde/hydroxyethylmethacrylate (HEMA) combination products such as G5™ All-Purpose Desensitizer (Clinician’s Choice Dental Products, Inc, www.clinicianschoice.com), Microprime G Desensitizing Agent (Danville Materials, www.danvillematerials.com), Gluma® Desensitizer PowerGel (Heraeus Kulzer, www.heraeus-kulzer-us.com), and Calm-It™ Desensitizer (DENTSPLY Caulk, www.caulk.com), to the dentin surface, multiple transverse septa occurred in the lumen of the dentinal tubules down to a depth of 200 µm (0.2 mm). This demonstrated that the combination products effectively create a barrier that eliminates the hydrodynamic mechanism of dentin hypersensitivity. The protein plug in the tubules also decreases the propensity for the negative effects of fluid flow on the ability to bond to the dentin substrate. Glutaraldehyde/HEMA desensitizer products also cross-link collagen (exposed during etching), which results in increased strength and durability of the hybrid layer resin dentin bonds.3
The HEMA component of these solutions, which is very hydrophilic, acts as a pre-primer to help facilitate resin infiltration of the exposed collagen, and thereby improve the longevity of the bond.4 Because these glutaraldehyde/HEMA products also contain water, they act as re-wetting agents. In the case of etch-and-rinse bonding procedures, the “re-wetting after the acid etch acts to expand the demineralised collagen and increase its surface energy, facilitating the diffusion of the hydrophilic resin monomer into the etched dentin.”5 A further benefit of using glutaraldehyde/HEMA combinations is that these products have antibacterial and anti-caries effects.6
Combining the primer and adhesive in the same mixture, as with the fifth-generation bonding agents as well as the seventh generation, places a hydrophilic compound together with a hydrophobic compound, which is problematic, because these two compounds are antagonistic, and, as Pashley states, they tend to be more permeable to water derived from the underlying dentin.7-9 One way to address this permeability is to decrease the fluid flow by the glutaraldehyde/HEMA products mentioned above, but an additional benefit can be derived by the addition of a hydrophobic, radiopaque, flowable composite liner like De-Mark (Cosmedent Inc., www.cosmedent.com), before placement of the final restoration. A hydrophobic layer not only decreases permeability,10,11 acting similarly to the last adhesive layer placed in the three-step etch-and-rinse bonding procedure, but it also gives the added benefit of the “elastic bonding” concept, acting as a stress breaker,12-14 while creating a radiopaque liner beneath the final restoration that cannot be misdiagnosed as caries.
The self-etch systems, or sixth-generation adhesives, are classified into two types. Type I adhesives, which are self-etch priming systems such as Clearfil™ SE Bond (Kuraray America, Inc. Dental, www.kuraraydental.com), Prelude SE (Danville Materials), and Ultradent Peak™ SE (Ultradent Products Inc., www.ultradent.com), use a self-etching primer followed by the application of an adhesive. These systems are gaining in popularity due to the fact they are not as clinically technique-sensitive, and are easy to use,15 with less reported post-operative sensitivity. However, controlled clinical studies show no difference in postoperative sensitivity as compared with etch-and-rinse systems when proper clinical protocol is used.16,17
With most of the self-etch systems, the clinician may sacrifice marginal seal and longevity.18,19 In order for a self-etch system to provide a good enamel marginal seal, the pH must be lower than 1.5 to effectively condition uncut enamel, and prevent marginal leakage; however, some of these products are mildly acidic, having a pH as high as 3.3. The research literature is replete with studies showing that these self-etch adhesives have more marginal defects,20 poor penetration with less adhesion,21 and increased microleakage22 in enamel when compared to etch-and-rinse systems, with a somewhat better result with instrumented enamel.23,24 This is worrisome because the enamel bond helps to protect the dentin bond from long-term degradation. Some clinicians still incorporate the use of a phosphoric acid on the enamel margins when using a self-etch product to enable increased bonding to the enamel.25 Using this technique, the clinician achieves a more predictable bond on the enamel margin; however, depending on control of the phosphoric acid, this technique can lead to clinical variability, and/or more permeability of the bond and sensitivity. The reason self-etch systems tend to minimize postoperative sensitivity is that the smear layer on the dentin surface and smear plugs in the dentinal tubules are left intact. If the phosphoric acid migrates onto the dentin surface during placement or the washing step, it can remove the smear layer and plugs, which allows fluid movement within the tubule; this leads to decreased tensile bond strength and sensitivity.26
If this is a preferred technique, the clinician may want to consider a phosphoric acid such as Ultra-Etch (Ultradent), which has the ideal viscosity for placement on vertical surfaces without migration. A recognized variable in the self-etch systems is the thickness of the smear layer, with diamond burs creating a thicker smear layer than carbide burs, resulting in less adhesion to dentin when the thick smear layer cannot be fully penetrated by the self-etch system.27,28 The self-etching primers, which are not rinsed off, are an acidic monomer, which may not be fully neutralized; this creates a demineralized zone below the hybrid layer that can compromise bond strength.29 A concern with self-etch systems is that they may not have resin penetration into or obturate the dentin tubules, thus allowing pulpal fluids to penetrate past the smear plug and into the hybrid layer.30 “The higher the micropermeability, the higher the risk of defects at the resin–dentin interface, which may represent the pathway for hydrolytic and enzymatic degradation of the collagen and resin dentin bonds over time.”31 This causes what is known as a “hydrolytic” or “water-tree” effect, which breaks downs the bond from the inside out, reducing both in-vivo and in-vitro bond strengths.32
As a general rule, self-etching systems are more ideally used in posterior restorations for prevention of sensitivity. In addition, due to a less predictable bond to enamel, which can lead to additional staining secondary to microleakage, these self-etch systems are not ideal for anterior restorations. When the level of enamel etching is of concern (ie, the pH is above 1.5), phosphoric-acid–etching may be indicated. However, some of these Type I adhesives, such as Peak SE, which has the highest bond strength in this category of 50 MPa to dentin,33 has an adhesive, Peak™ LC Bond Resin (Ultradent), that can be used in the anterior dentition with an etch-and-rinse phosphoric-acid technique. Many of these products do have catalysts for use with dual-cured composites and can be compatible with self-cure.
Type II self-etch adhesive systems such as All-Bond SE® (BISCO, Inc., www.bisco.com), Brush & Bond® (Parkell, www.parkell.com), Futurabond® NR (VOCO America, Inc., www.vocoamerica.com), Touch & Bond® (Parkell), Adper™ Prompt™ L Pop™ (3M ESPE, www.3mespe.com), and Xeno III® (DENTSPLY Caulk), use a self-etch primer and adhesive that are mixed together prior to placement. These self-etching primer/adhesives should not be confused with the self-etching primers of Type I systems. Both Type I and Type II systems leave the smear layer intact before placement and thereby limit postoperative sensitivity. However, Type II systems have all of the same drawbacks as Type I, and can have 35% lower bond strength, because no hydrophobic adhesive layer is placed. As mentioned above, the hydrophobic resin layer helps to prevent water-induced interfacial changes.34 It is important to note that thermocycling, which is used to more closely mimic oral conditions, leads to further lowering of the bond strength of these hydrophilic systems.35 The remaining acidity and permeability of these Type II products make them incompatible with self- or dual-cured composites and core materials. Touch & Bond, for instance, demonstrates extremely low bond strengths of 12 MPa to enamel and only 2 MPa to dentin.36
Among the self-etch adhesives—also called “all-in-one” or seventh-generation adhesive systems—are G-Bond™ (GC America, www.gcamerica.com), iBond® (Heraeus Kulzer, www.heraeus-dental-us.com), Xeno® IV (DENTSPLY Caulk), Adper™ Easy Bond (3M ESPE), AdheSE® One (Ivoclar Vivadent, www.ivoclarvivadent.com), and Clearfil® S3 Bond (Kuraray). They are very similar to sixth-generation systems, with the biggest difference being that all the components are pre-mixed in one bottle. This one-bottle solution etches, primes, and bonds all at the same time. These self-etch adhesives are permeable membranes and are the most hydrophilic of the adhesive categories.37 As such, water sorption by polymers (composites) causes plasticization and lowers mechanical properties.38 Residual acidity causes an adverse reaction with chemically cured composites and core materials, creating a reduction in bond strength with permeability, also a further cause of bond strength reduction.39 Swift states that for these single-step self-etch adhesives, the bond strength to chemical-cured composites can be enhanced with the adjunctive use of co-initiators, based on sodium salts of aromatic sulphinic acids, but he notes that it might not apply to all simplified adhesives.40 This generation of self-etch adhesives also has the highest pH values which results in one-fifth the bond strength to enamel versus the three-step etch-and-rinse system,41 and a higher percentage of leakage at the margins.42 In general, the all-in-one seventh-generation bonding agents show lower bond strengths, with G-Bond having a bond strength of 12.5 MPa to dentin and 15.4 MPa to enamel.33
It is well known that intraoral, in-vivo bonding of composite resin to dentin decreases with the age of the restoration.43 Bonding stability is affected negatively by factors such as permeability, lack of full penetration of the bonding agent to the full depth of the etched dentin, and the etching process itself (etch-and-rinse or self-etch). Etching dentin results in a superficial exposure of the collagen fibers and other collagen-associated proteins. Subsequent use of the dental adhesive system allows resin infiltration of the collagen and results in the formation of the hybrid layer. Degradation of collagen fibers associated with the hybrid layer by proteolysis results in a gradual reduction in dentin bond strengths.44 The end result of the collagen degradation is the loss of continuity between collagen fibrils in the hybrid layer and the underlying mineralized matrix into which they are anchored. This eventually leads to lower bond strengths, increased nanoleakage, and dentin/pulpal sensitivity, and it ultimately leads to the replacement of the restoration sooner than expected. Matrix metalloproteinases (MMPs) are among other collagen-associated proteins exposed by the etching process and can slowly degrade collagen in the hybrid layer.45 As well, it is thought that mildly acidic monomers present in dental adhesives can activate MMPs, making them prone to degrade the acid-etched, unprotected collagen fibers.46 Early reports have shown that glutaraldehyde cross-links fibers, making it more difficult for the collagen-associated MMPs to break down the collagen fibers associated with the hybrid layer.47 In this way, glutaraldehyde is able to help establish a more stable hybrid layer. Other protein cross-linking agents are currently being investigated. MMP inhibitors such as chlorhexidine show promise for initial stabilization of the hybrid layer.48-53 In response to this ongoing investigation and work on stabilizing the long term-bond, Peak™ LC Bond Resin has recently added chlorhexidine to its formulation.
Making a decision on a suitable dental adhesive is not easy, as there are many factors to consider. The driving factor should be choosing the product and/or procedure that will offer the best quality of care for patients, and deliver the most predictable long term-results. The predictability of fourth- and fifth-generation adhesives has been unmatched. Ongoing research may lead to advances in dental chemistry that result in stable, long-term attachment to both enamel and dentin.
Dr. Boksman was previously a part-time paid consultant to Clinician’s Choice and Clinical Research Dental, holding the title of Director of Clinical Affairs.
1. Boksman L. Glutaraldehyde/HEMA: A review of the literature. Dentistry Today. 2009;30(9):60-65.
2. Shüpbach P, Lutz F, Finger WJ. Closing of dentinal tubules by Gluma desensitizer. Eur J Oral Sci. 1997;105(5 Pt 1):414-421.
3. Bedran-Russo AK, Pashley DH, Agee K, et al. Changes in stiffness of demineralised dentin following application of collagen cross-linkers. J Biomed Mat Res B App Biomater. 2008;86(2):330-334.
4. Xu J, Stangel I, Butler IS, Gilson DF. An FT-Raman spectroscopic investigation of dentin and collagen surfaces modified by 2-hydroxyethylmethacrylate. J Dent Res. 1997;76(1):596-601.
5. Bansal A, Shivanna V. Effect of wetting agents on the shear bond strength of different bonding agents when applied to dry dentin. J Cons Dent. 2007;10(1):26-32.
6. Felton D, Bergenholtz G, Cox CF. Inhibition of bacterial growth under composite restorations following Glum pre-treatment. J Dent Res. 1989;68(3):491-495.
7. Tay FR, Pashley DH. Have dentin adhesives become too hydrophilic? J Can Dent Assoc. 2003;69(11):726-731.
8. Tay FR, Pashley DH, Suh BI, et al. Single-step adhesives are permeable membranes. J Dent. 2002;30(7-8):371-382.
9. Tay FR, Frankenberger R, Krejci I, et al. Single-bottle adhesives behave as permeable membranes after polymerization. I. In vivo evidence.J Dent. 2004;32(8):611-621.
10. Van Meerbeek B, Willems G, Celis JP, et al. Assessment by nano indentation of the hardness and elasticity of the resin-dentin bonding area. J Dent Res. 1993;72(10):1434-1442.
11. Powers JM, O’Keefe KL, Pinzon LM. Factors affecting in vitro bond strength of bonding agents to human dentin. Odontology. 2003;91(1):1-6.
12. De Munck J, Van Meerbeek B, Yoshida Y, et al. Four year water degradation of total-etch adhesives bonded to dentin. J Dent Res. 2003;82(2):136-140.
13. Van Meebeek B, Peumans M, Vershueren M, et al. A clinical status of ten dentin adhesive systems. J Dent Res. 1994;73(11):1690-1702.
14. Li Q, Jepson S, Albers HK, Eberhard J. Flowable materials as an intermediate layer could improve the marginal and internal adaptation of composite restorations in Class-V cavities. Dent Mater. 2006;22(3):250-257.
15. Loguercio AD, Bittencourt DD, Baratieri LN, Reis A. A 36-month evaluation of self-etch and etch-and-rinse adhesives in non-carious cervical lesions. J Am Dent Assoc. 2007;138(4):507-514.
16. Browning WD, Blalock JS, Callan RS, Brackett WW, et al. Postoperative sensitivity: a comparison of two bonding agents. Op Dent. 2007;32(2):112-117.
17. Casselli DS, Martins LR. Postoperative sensitivity in Class I composite resin restorations in vivo. J Adhes Dent. 2006;8:53-58.
18. Kanemura N, Sano H, Tagami J. Tensile bond strength to and SEM evaluation of ground and intact enamel surfaces. J Dent. 1999;27(7);523-530.
19. Pashley DH, Tay FR. Aggressiveness of contemporary self-etching adhesives. Part II: etching effects on un-ground enamel. Dental Mater. 2001;17(5):430-444.
20. Van Meebeek B, Kanumilli P, De Munck J, et al. A randomized controlled study evaluating the effectiveness of a two-step self-etch adhesive with and without phosphoric acid etching. Dent Mater. 2005;21(4):375-383.
21. Hashimoto M, Ohno H, Yoshida E, et al. Resin enamel bonds made with self-etching primers on ground enamel. Eur J Oral Sci. 2003;111(5):447-453.
22. Deliperi S, Bardwell DN, Wegley C. Restoration interface microleakage using one total-etch and three self-etch adhesives. Oper Dent. 2007;32(2):179-184.
23. Brackett WW, Ito S, Nishitani Y, et al. The microtensile bond strength of self-etching adhesives to ground enamel. Oper Dent. 2006;31(3):332-337.
24. Perdigao J, Geraldeli S. Bonding characteristics of self-etching adhesives to intact versus prepared enamel. J Esthet Restor Dent. 2003;15(1):32-42.
25. Van Meebeek B, Kanumilli P, De Munck J, et al. A randomized controlled study evaluating the effectiveness of a two-step self-etch adhesive with and without selective phosphoric etching of enamel. Dent Mater. 2005;21(4):375-383.
26. Torii Y, Itou K, Nishitani Y, et al. Effect of phosphoric acid etching prior to self-etching primer application on adhesion of resin composite to enamel and dentin. Am J Dent. 2002;15(5):305-308.
27. Ogata M, Harada N, Yamaguchi S, et al. Effects of different burs on dentin bond strengths of self-etching primer bonding systems. Oper Dent. 2001;26(4):375-382.
28. Kenshima S, Reis A, Uceda-Gomez N, et al. Effect of smear layer thickness and pH of self-etching adhesive systems on the bond strength and gap formation to dentin. J Adhes Dent. 2005;7(2):117-126.
29. Oliveira SS, Marshall SJ, Habelitz S, et al. The effect of a self-etching primer on the continuous demineralization of dentin. Eur J Oral Sci. 2004;112(4):376-383.
30. Radovic I, Vulicevic ZR, Garcia-Godoy F. Morphological evaluation of 2- and 1-step self-etching system interfaces with dentin. Op Dent. 2006;31(6):710-718.
31. Sauro S, Pashley DH, Mannocci F, et al. Micropermeability of current self-etching and etch-and-rinse adhesives bonded to deep dentine: a comparison study using a double-staining/confocal microscopy technique. Eur J Oral Sci. 2008;116(2):184-193.
32. Donmez N, Belli S, Pashley DH, Tay FR. Ultra-structural correlates of in vivo/in vitro bond degradation in self-etch adhesives. J Dent Res. 2005;84(4):355-359.
33. Christensen GJ. Bonding agents: Is convenience overriding strength? Clinician’s Report. 2010;3(6):1-3.
34. Carvalho RM, Pegoraro TA, Tay FR et al. Adhesive permeability affects coupling of resin cements that utilize self-etching primers to dentine. J Dent. 2004;32(1):55-65.
35. Kerby RE, Knowbloch LA, Clelland N, et al. Microtensile bond strengths of one-step and self-etching adhesive systems. Oper Dent. 2005;30(2):195-200.
36. Farah JW, Powers J. Bonding agents. The Dental Advisor. 2007;24(6):1-40.
37. Van Landuyt KL, Mine A, De Munck J, et al. Technique sensitivity of water-free one-step adhesives. Dent Mater. 2008;24(9):1258-1267.
38. Ito S, Hashimoto M, Wadgaonkar B, et al. Effects of resin hydrophilicity on water sorption and changes in modulus of elasticity. Biomaterials. 2005;26(33):6449-6459.
39. Tay FR, Pashley DH, Yiu CK, et al. Factors contributing to the incompatibility between simplified-step adhesives and chemical-cured or dual-cured composites. Part 1. Single-Step self-etch adhesive. J Adhes Dent. 2003;5(1):27-40.
40. Carvalho RM, Garcia FCP, e Silva SMA, et al. Adhesive-composite incompatibility, Part II. J Adhes Dent. 2005;17(3):191-195.
41. De Munck J, Van Meerbeek B, Satoshi I, et al. Microtensile bond strengths of one- and two-step self-etch adhesives to bur-cut enamel and dentin. Am J Dent. 2003;16(6):414-420.
42. Ernst CP, Cortain G, Spohn M, et al. Marginal integrity of different resin-based composites for posterior teeth: an in vitro dye-penetration study on eight resin-composite and compomer/adhesive combinations with a particular look at the additional use of flow-composites. Dent Mater. 2002;18(4):351-358.
43. Hashimoto M, Ohno H, Kaga M, et al. In vivo degradation of resin-dentin bonds in humans over 1 to 3 years. J Dent Res. 2000;79(6):1385-1391.
44. Sano H, Yoshikawa T, Periera PN. Long-term durability of dentin bonds made with a self-etching primer, in vivo. J Dent Res. 1999;78(4);906-911.
45. Zhang S-C, Kern M. The role of host-derived dentinal matrix metalloproteinases in reducing dentin bonding of resin adhesives. Int J Oral Sci. 2009;1(4):163-176.
46. De Munck J, Van den Steen PE, Mine A, et al. Inhibition of enzymatic degradation of adhesive-dentin interfaces. J Dent Res. 2009;88(12):1101-1106.
47.Cheung DT, Tong D, Perelman N, et al. Mechanism of crosslinking of proteins by glutaraldehyde IV: in vitro and in vivo stability of a cross-linked collagen matrix. Connect Tissue Res. 1990;25(1):27-34.
48. Pashley DH, Tay FR, Breshi L, et al. State of the art etch-and-rinse adhesives. Dent Mater. 2011;27(1):1-16.
49. Carrilho MR, Carvalho RM, de Goes MF, et al. Chlorhexidine preserves dentin bond in vitro. J Dent Res. 2007;86(1):90-94.
50. Carhillo MR, Geraldeli S, Tay FR, et al. In vivo preservation of the hybrid layer by chlorhexidine. J Dent Res. 2007;86(6):529-533.
51. Hebling J, Pashley DH, Tjaderhane L, Tay Fr. Chlorhexidine arrests subclinical degradation of dentin hybrid layers in vivo. J Dent Res. 2005;84(8):741-746.
52. Suh Bi, Chen L, Brown DJ. A novel concept: The introduction of cross-linking monomers into a self-etch adhesive to create a more hydrophobic & durable bond. Oral Health Group. 2011;62-94.
53. Moon PC, Weaver J, Brooks C. Review of matrix metalloproteinases effect on the hybrid dentin bond layer stability and chlorhexidine clinical use to prevent bond failure. Open Dent J. 2010 July 20;4:147-152.
About the Authors
Leendert (Len) Boksman, DDS, BSc, FADI, FICD
Retired from Private Practice
London, Ontario, Canada
Gregg Tousignant, CDT
Technical Support Manager
Clinical Research Dental
London, Ontario, Canada
Lee W. Boushell, DMD, MS
Department of Operative Dentistry
University of North Carolina School of Dentistry
Chapel Hill, North Carolina
Gildo Coelho Santos, Jr., DDS, MSc, PhD
Assistant Professor and Chair Division of Restorative Dentistry
Schulich School of Medicine and Dentistry
University of Western Ontario
London, Ontario, Canada
London, Ontario, Canada